DOI 10.1617/s11527-006-9111-2 O R I G I N A L A R T I C L E

**Pull-out strength of axially loaded steel rods bonded**

**in glulam parallel to the grain**

**R. Steiger****· E. Gehri · R. Widmann**

Received: 8 June 2005 / Accepted: 15 November 2005 / Published online: 19 October 2006 C

RILEM 2006

**Abstract Bonded-in steel rods are very efficient in**
withstanding high forces applied to timber members.
Investigations of bonded-in rods started in the late
eighties of the last century and several design models
were published since. By comparing these approaches
on base of an extensive literature review a certain
de-gree of discrepancy and partly even contradiction can
be found. The paper describes a test program which
aimed to study the influence of timber density and of
geometric parameters on the pull-out strength of
sin-gle axially loaded steel rods. Following the GSAR
-procedure, which is a well established glued-in rods
joint in Switzerland, rods with metric thread were
bonded in glulam made of Norway spruce lamellas
us-ing an epoxy-type adhesive. The tests showed that the
influence of the timber density can be quantified by a
power function of*ρ with an exponent of 0.6. The *
pa-rameters length of the glued zone * and diameter of*
*the hole dH* can be summarized in the slenderness
ra-tio*λ = /dH*, which itself is related to the mean shear
strength in the anchoring zone by an exponent of
ap-proximately −1/3. In order to prevent the specimens
from premature splitting, distances between the axis of

R. Steiger (_{})· R. Widmann

Empa, Swiss Federal Laboratories for Materials Testing and Research, Wood Laboratory, ¨Uberlandstrasse 129, CH-8600 D¨ubendorf, Switzerland

e-mail: rene.steiger@empa.ch E. Gehri

Prof. em. ETH, CH-8803 R¨uschlikon, Switzerland

the rod and the edge of the specimen of 2.3 times the diameter of the rod have been used.

**R´esum´e En utilisant des tiges nervur´ees coll´ees il est**

*possible d’appliquer des grands charges `a des ´el´ements*
*constructifs en bois. Comme r´esultat de l’exploration*
*des barres m´etalliques encoll´ees, qui ´etait commenc´ee*
*`a la fin des ann´ees quatre-vingts du dernier si`ecle,*
*plusieurs propos de calcul ont ´et´e publi´e. En comparant*
*ces propos de calcul trouv´es en cours d’une recherche*
*´etendue de la litt´erature, une certaine divergence et de*
*temps en temps mˆeme contradiction peuvent ˆetre *
*con-stat´ees. L’article-ci d´ecrit une s´erie d’essais en cours*
*de laquelle on voulait examiner l’influence de la *
*den-sit´e du bois et de diff´erents param`etres g´eom´etriques*
*sur la r´esistance `a la traction axiale d’une seule*
*tige. Les tiges avec filetage m´etrique ont ´et´e coll´ees*
*dans du bois lamell´e-coll´e d’´epic´ea avec une r´esine*
*´epoxy selon la proc´edure GSA*R *qui repr´esente un*
*syst`eme bien ´etabli en Suisse. Les essais ont montr´e*
*que l’influence de la densit´e du bois peut ˆetre *
*quan-tifi´ee par une fonction potentielle avec un exposant de*
*0.6. La longueur de la zone coll´ee et le diam`etre du*
*trou dH, r´eunis comme ´elancement relativeλ = /dH,*

*sont en rapport avec la r´esistance au cisaillement*
*moyenne de la longueur d’encollage avec un exposant*
*de−1/3. Afin d’´eviter un fendillement pr´ematur´e dans*
*le bois des distances de 2.3 fois le diam`etre de la*
*tige entre son axe et le bord du sp´ecimen ont ´et´e*
*r´ealis´ees.*

**Keywords Glued-in steel rod . Glulam . Pull-out**
strength . Parallel to the grain . Parameter study .
Epoxy

**1. Introduction**

Steel rods bonded in glulam elements are very effi-cient joints that can withstand high axial forces applied to timber structural members. Research on bonded-in rods started in the late eighties of the last century. At-tempts to develop design methods that would optimize the application of such joints were intensified within the last 10 years [1–5].

Several design approaches and code models have
been published [6–10]. By comparing these models and
approaches on base of an extended literature review,
some discrepancy and partly even contradictions
be-tween the models, especially regarding the treatment of
isolated parameters, were found. On this background,
a test program was initiated to study the influence of
a selection of these parameters, known or supposed to
be determinant on the pull-out strength of single,
axi-ally loaded steel rods. Test specimens consisted of rods
with a metric screw-thread, bonded with an epoxy-type
adhesive into glulam made of Norway spruce (Fig. 1).
The tests were focused to determine the influence of
timber density*ρ, length and diameter d of the rod (or*
*the corresponding drill-hole dh*respectively) and of the
distances between the axis of the rod and the edge of
the specimen on the pull-out strength of the rod.

Important objectives of the test program were that it should be based on practically applicable situations and dimensions and that it should enable a comparison with similar test series. These objectives could only be reached by permitting certain compromises regarding

**Fig. 1 Geometry of specimens (dimensions see Tables 1 and 2)**

the test layout. Although for example in practice the use of one single rod will not or hardly ever be the normal case, all tests described here were carried out on connections with one single rod, because the exam-ination of such a connection provides a good basis to study the influence of the parameters mentioned before. In practice the tested GSAR-system [11] is optimized in such way that yielding of the steel rod is decisive, thus resulting in a ductile behaviour of the joint. Con-trary to practice the aim of the study was to analyse the influence of timber-related parameters on the pull-out strength of the rods. Therefore rods of high yield limit and strength were chosen, in order to provoke shear failure in the timber.

Although the test results and the conclusions are specifically valid for the tested system and loading con-figuration, it is possible to draw some general conclu-sions about the quantification of the influence of the parameters focused by the study and to propose an ad-equate strength model.

**2. Review of existing approaches**
2.1. Influence of timber density

Since most of the mechanical properties of timber (of
the same species) are known to be more or less directly
related to the density of the timber, it is to be supposed
that the pull-out strength of glued-in steel rods also
depends on the timber density, provided steel yielding
and cohesive or adhesive failure are avoided. For screws
and screw nails set in timber perpendicular to its grain,
the influence of the density on the pull-out strength was
demonstrated for example by [12–15] and was taken
into account by a power function of the density (*ρc*_{)}
*with exponents c up to 2.5 [12].*

Compared to screws and screw nails, glued-in rods introduce the shear forces into the timber in a differ-ent way. While the “anchored” screws rely on direct contact between the timber and the flanks of the thread and therefore on a kind of compression of complex ge-ometry, the glued-in rods transfer the force only at the interface between the rod and the adhesive. The load transfer between the adhesive and the timber is gov-erned mainly by shear and not by compression due to indentation. Being aware of this, a dependence of the pull-out strength of glued-in rods on the timber density can be expected. However this influence should be less

significant compared to screws and screw nails because the shear strength of timber is affected by the density to a lesser degree than its compression strength.

Researchers have stated different opinions on the
in-fluence of the timber density on the pull-out strength
of glued-in rods. While some of them (for example:
[16, 17]) derived such an influence from their test
re-sults, others asserted the pull-out strength to be
inde-pendent of timber density [18] or to exhibit poor
cor-relation [8, 19, 20]. Design models derived from the
tests take into account the influence of density by power
functions*ρcwith exponents c in the range of 0 to 1.5*
according to the rod-to-grain angle [6, 8–10, 20–24].
All of these design models consider the dependence on
the density, if taken into account at all, to be marked
more for rods set in parallel to the grain, than for those
set perpendicular to the grain.

2.2. Influence of length and diameter of the anchoring zone

The diameter and the length of the rod or of the hole
respectively (which is a better way of analysing data
derived from tests with clear failure in the timber) were
shown by different studies (for example by [8, 10, 16,
21, 23, 25, 26]) to be the dominant influence on the
pull-out strength of glued-in rods. The glued length* + _{v}*
(

*corresponds to the anchoring length, where the load*is actually transmitted from the rod to the timber; the length

*is a tapered portion of the rod without any load transfer capacity (Fig. 1)). The anchoring length*

_{v}*and the diameter dh*of the drill-hole can be combined in a single parameter called slenderness ratio

*λ = /dh*. In [8] a very strong effect of absolute size of the rod and also of the rod’s slenderness is presented for brittle adhesives.

2.3. Influence of the rod’s distances to the edge of the specimen

In order to prevent the timber from early splitting due
to tensile stresses perpendicular to the grain, which
is part of the multiaxial stresses within the anchoring
zone, minimal distances between the rod and the edge
of the specimen have to be provided. Early studies on
glued-in rods were performed with edge distances of
4*·d [16, 25]. Although sometimes this value was used*
again later on [8], most of the latest design approaches

and experimental studies use distances of 2.5*·d between*
the axis of the rod and specimen’s edge [9, 27, 28].

With regard to an optimal performance of the joint
in terms of resulting tensile stress in the timber net
cross-section the edge distances should be as small as
possible. The GSAR-system tested in the course of this
study, uses edge distance ratios of 2.3·d to 2.4·d. In
[29] it was reported, that edge distance ratios of 1.5*·d*
resulted in premature splitting of the timber, whilst this
was not the case for edge distance ratios*≥2·d.*

**3. Tests**

3.1. Material properties

*3.1.1. Timber*

The specimens were cut from glued-laminated tim-ber made of Norway spruce lamellas of 40 mm thick-ness. The lamellas were free from any finger-joints or significant anatomical defects such as big knots and deviations of grain angle, in order to avoid negative influence on the results by these parameters. The glu-lam members were assembled using a meglu-lamine urea formaldehyde (MUF) adhesive. Two pairs of glulam beams were produced from lamellas with clearly dis-tinct distributions of density (Fig. 2 and Table 3), in order to quantify the influence of the timber density on the pull-out strength of the rods. Every single specimen was cut from a beam with a desired density respectively.

**Fig. 2 Box-plots of lamellae’s densities***ρ*0 used for the four
glulam beams which served as base for the production of the
specimens

*3.1.2. Adhesive*

The rods were set using a system called GSAR by
n’H (Neue Holzbau AG, Switzerland) [11]. For the
GSAR-system a special epoxy-type adhesive, free
from any solvent and curing at ambient temperature
has been developed by ASTORit AG, Switzerland.
This adhesive performs well, as company internal tests
showed. Shear strengths up to 35 N/mm2_{were reached}
between two threaded steel surfaces bonded together.
Tests on threaded steel rods bonded in ash established
shear failure in timber at nominal shear strength levels
of 16 to 18 N/mm2.

*3.1.3. Steel rods*

In practice, joints with glued-in rods should be designed
in such way that steel failure (yielding) occurs (Fig. 3)
and not wood- or adhesive failure in order to achieve a
ductile rather than a brittle rupture. The GSAR-system
considers this fact by reducing the cross-section of the
steel rods within a certain length * _{v}*, based on an
in-vestigation by Fabris [30]. Removing the rod’s thread
within the length

*v*also leads to a shift of the anchoring zone to the interior of the specimens. Stress concentra-tions are reduced and splitting due to shear forces and stresses perpendicular to the grain are less likely to hap-pen [26, 30, 31]. The drill-hole was filled with glue on its whole length

*+*. However, it was assumed that the zone along the length

_{v}*v*can not contribute to the pull-out resistance due to the lack of mechanical inden-tation of rod and adhesive. The length

*was taken to be 5*

_{v}*·d.*

The steel rods with metric threads M12, M16 and M20 were zinc coated and corresponded to quality 8.8

**Fig. 3 Steel failure (yielding of the rod)**

**Fig. 4 Shear failure in timber**

*(nominal yielding point: fy*≈ 640 N/mm2_{/}_{ε}

*y*≈ 3‰ and
*nominal ultimate tensile strength: fu* ≈ 800 N/mm2_{).}
This high-quality steel was chosen in order to
pro-voke timber shear failure (Fig. 4) rather than steel
failure (Fig. 3). The rods were set in holes with
*diameters dh* that exceeded the rod diameter by
2 mm.

3.2. Specimens, equipment and procedure

*3.2.1. Specimens*

The rods set parallel to the grain were tested in a
double-ended (pull-pull) configuration (Fig. 5). In
or-der to give the joints an optimal performance both the
timber and the steel elements should have a similar
*stiffness (A*Timber *· E*Timber *≈ A*Steel *· E*Steel*), A being*
*the cross-section and E the modulus of elasticity [26,*
*30]. The ratio A*Timber*/A*Steelshould therefore be equal to

**Table 1 Geometric**
properties of specimens in
reference to Fig. 1
Series *d−dh*[mm] *a [mm]* *v*[mm] * [mm]* *λ = /dh* tot[mm]
M12 12–14 55 60 105 7.5 580
140 10 650
175 12.5 720
210 15 780
M16 16–18 75 80 140 7.78 700
175 9.72 780
220 12.2 880
270 15 970
M20 20–22 95 100 175 7.96 980
220 10.0 1070
275 12.5 1180
330 15 1240
**Table 2 Geometric**

properties of specimens for evaluation of cross-section in reference to Fig. 1

Series *d− dh*(mm) * (mm)* *v*(mm) tot(mm) *a (mm)* *e= 0.5·a/d*

M16 16–18 175 80 780 56 1.75 65 2.03 75 2.34 85 2.66 100 3.13 120 3.75

*the ratio E*Steel*/E*Timberwhich is approximately 16 to 20
for Norway spruce. From the practical point of view,
*high ratios of A*Timber */ A*Steel are unattractive because
of a poor performance of the joint itself, regarding the
resulting tensile stress in the glulam element. However,
in order to prevent early splitting of timber due to stress
concentrations, the cross-sections of the specimens had
to be designed in such way that edge distance ratios
from 2.3*·d to 2.4·d resulted and this represented ratios*
*of A*Timber*/A*Steelfrom 37 to 39. Geometry and
dimen-sions of the specimens are shown in Table 1 and in Fig.
1. In general there were four specimens per each
com-bination of rod diameter, timber density and anchoring
length resulting in a total number of 96 specimens with
192 glued-in rods.

In order to study the influence of the distance be-tween the rod and the edge of the specimen, a supple-mentary series of 24 specimens (48 rods) with edge distance ratios between 1.75·d and 3.75·d was addi-tionally tested (Table 2).

*3.2.2. Equipment and procedure*

All tests were carried out on a universal tension testing machine (Fig. 5) with a maximal error of the force

**Table 3 Sample statistics of lamellae’s densities**

Density*ρ*0(kg/m3)
Parameter Low 1 High 1 Low 2 High 2

*Sample size n* 12 12 12 12
Mean value 371 493 378 498
Maximum 388 508 390 515
Minimum 353 481 365 492
Standard deviation 13.2 10.8 8.38 7.67
Coeff. of variation 3.6% 2.2% 2.2% 1.5%
*ρk*a 349 475 364 485

a_{5th percentile assuming normal distribution and n}_{= ∞}

measurement*<1%. The rate of loading was taken in*
accordance with EN 26891 [32].

**4. Results and discussion**
4.1. General

An overview of the test results is given in Fig. 6. Even though it was only verified by spot checks, there was strong evidence that the pull-out of the rods occurred due to shear failure of the wood around the anchoring zone of the rods (Fig. 4). Visible splitting and cracking

**Fig. 6 Overview of ultimate loads Fu**. (Maximum, Mean,

*Minimum). Number of specimens n*= 4 for all series except
for*<M16-270 L&H> and <M20-330 L> with n = 3. Values*
for series*<M12-210> include steel failures or wood-tension*
failures

**Fig. 7 Tensile failure in timber**

at the ends of the specimens occurred at about 65% of
all tests. However, there were no significant differences
between the failure loads of specimens with and
with-out external signs of cracking/splitting. Cracking
there-fore did not influence the pull-out strengths and was
regarded as being a consequence of the internal shear
failure of the wood. The rupture of three out of the
four specimens *<M12-210 High density> occurred*
due to steel failure and within the series *<M12-210*

*Low density> two out of the four specimens showed*

tension failure in timber on a very low strength level (Fig. 7). Since the failure mode of these specimens was different to that aimed at in the strength model, both series were excluded from further analysis. (Timber tensile failure in practice has to be avoided by ade-quate quality control of the glulam members used for structural purposes.)

The recorded ultimate loads of series M20 (low den-sity) and M16 (both low and high denden-sity) with the longest anchoring lengths had significantly higher co-efficients of variation compared to all other series. In all three series mentioned this was due to one single low value. Investigations on this showed significantly tilted positions of the respective rods which caused ec-centric loading. It was decided to take no account of these single values at the following analysis.

In general Fig. 6 gives a good impression on the influence of timber density, rod diameter and rod length on the pull-out-strength of the rods. The influence of these individual parameters is looked at in greater detail in the following.

4.2. Influence of timber density

Within every series with identical geometrical
*proper-ties, the mean value of the pull-out strengths Fu _{,mean}*
of the specimens with a high wood density was
signif-icantly higher than that of the specimens with a low
wood density. The mean ratio of high density wood
(H) to low density wood (L) was found to be

*ρH*/

*ρL*= 1.33. The ratio of the respective mean ultimate loads

*Fu,H/Fu,L*varied from 1.11 to 1.28 with a mean value of
1.18. As only high and low density samples were tested,
no statement to the progression of density ratio*ρH*/*ρL*
*against load ratio Fu _{,H}/Fu,L* could be made on base of
the test results. In literature often a power function is
given to describe their dependency. On this base a mean

*value of the exponent c*mean

*= 0.60 for (Fu,H/Fu,L*)= (

*ρH*/

*ρL)c*could be calculated. This value matches

*re-sults of other studies very well, indicating c= 0.55 for*epoxy-type adhesives [33] and at the same time rejects

*proposals of higher c-values.*

4.3. Influence of anchoring length and of drill-hole diameter

As already mentioned initially, the tests were planned
to follow a certain range of geometrical proportions in
*terms of drill-hole diameter dh*and anchoring length*,*
or in combination also represented by the slenderness
ratio*λ = /dh. Besides analysing the test results with*
regard to*λ, the influences of the individual parameters*
* and dh* were studied, in order to get an idea about
*their significance. The nominal shear strength f _{v,0,mean}*
was calculated assuming a constant distribution of the
shear stresses over the anchoring length

*. However,*

**Fig. 8 Nominal shear strength versus anchoring length. The**

dotted line represents the kind of progression if a dependence

*fv,0,mean*against (2*/*1)*−1/3*is assumed (2*> *1)

it is known from respective finite element simulations that in case of rods glued-in parallel to the grain, the stress distribution is uneven with peaks at both ends of the anchoring zone [20, 34, 35].

With increasing anchoring lengths the ultimate loads
also increased (Fig. 6) but the nominal shear strengths
decreased (Fig. 8). A reason for the decreasing shear
strengths is seen in the mentioned distribution of the
shear stresses along the rods length. For the description
of the dependency of shear strengths against anchoring
length an approach based on*−1/3*is suggested.

Regarding the influence of the slenderness ratio*λ =*
*/dh* *on the nominal shear strength fv,0,mean*, a power
function*λ−1/3*fits the test results well (Fig. 9).

The analysis of the influence of the drill-hole
diame-ter on nominal shear strength was based on the
compar-ison of series with similar anchoring lengths but
differ-ent hole- and rod diameters. In Fig. 6 it clearly appears
that ultimate loads increased with increasing
diame-ters. However, the influence of the drill-hole diameter
on the nominal shear strength could not be clearly
ver-ified (Fig. 10). For most of the series nominal shear
*strength increased with increasing diameter dh*but for
a glued length of* = 220 mm it decreased with an *
in-creasing diameter from M16 to M20.

Based on an approach *λ−1/3*, the influence of the
*hole-diameter dh* on the pull-out strength of rods set
*parallel to the grain needs to be dh*1*/3* _{if a constant}

**Fig. 9 Nominal shear strength versus slenderness ratio***λ = /dh*

**Fig. 10 Mean value of density-adjusted nominal shear strength**

*versus drill-hole diameter dh*for three different anchoring lengths

length is assumed. This could not be proved in detail on base of the test results.

In general it can be stated, that if the single
param-eters anchoring length* and diameter of the drill-hole*

*dh*are taken as a base for the determination of the
*pull-out strength f _{v,0,mean}* of rods set parallel to the grain,
both parameters would have to be put in consideration
and both with different exponents. An approach based
on the slenderness

*λ therefore seems to be the better*solution.

4.4. Influence of timber cross-section

In Fig. 11 it can clearly be seen, that for edge distance
ratios smaller than 2.3*·d the pull-out strength values*

**Table 4 Resulting tensile stress in wood**

(Mean value of sample means of ultimate
*loads Fu* for all series with*λ from 7.5 to*

12.5 and for both high and low density sam-ples)

Rods M12 M16 M20

*Mean Fu,mean*(kN) 43.8 77.2 110

*σt,0*(N/mm2_{)} _{14.5} _{13.7} _{12.2}

**Table 5 Resulting tensile stress in**

*wood (Max values of ultimate loads Fu*

for high density samples)

Rods M12 M16 M20

*MaxFu*(kN) 65.7a 121 164
*σt,0*(N/mm2_{)} _{21.7}a _{21.5} _{18.2}
a_{Steel failure (yielding of the rod)}

**Fig. 11 Influence of the rod’s distance to the edge of the **

speci-men

decreased significantly, which is in accordance with re-quests of most actual design approaches. Edge distance ratios smaller than 2.3·d therefore should be avoided in order to prevent premature splitting of the timber re-sulting in low pull-out strength values.

With regard to an optimal load transfer capacity of
the joint the timber cross-section should be as small as
possible. A comparison of the resulting tensile stresses
in the timber members shows, that for a given edge
dis-tance ratio of 2.3·d the load transfer capacity from steel
to timber was better for the smaller diameters (Table 4).
With regard to an optimal load transfer capacity
pref-erence therefore should be given to rods with smaller
diameter. For high density glulam and slenderness
ra-tio*λ = 15 maximum tensile stresses over 20 N/mm*2

**Fig. 12 Design model in comparison to density-adjusted (***ρ =*

480 kg/m3_{) mean values of test results}

were reached with respect to the timber cross-section (Table 5).

4.5. Pull-out strength model

The test results permit to propose a strength model
for the calculation of the pull-out strength on a mean
level. For wood density a reference value of*ρ*mean=
480 kg/m3 _{being near to the mean density of the high}
density samples serves as base. On the geometrical side
*λ = 10 which represents a value in the middle range*
of the tested geometries was chosen as reference base.
With the mean values of the test results adjusted to the
mentioned*λ and ρ, a corresponding shear strength of*
7.8 N/mm2results. Thus, the nominal shear strength of
single, axially loaded rods set parallel to grain results
in:
*f _{v,0,mean}= 7.8 N/mm*2

_{·}

*λ*10

*·*

_{−1/3}*ρ*480 0

*.6*

The pull-out strength thus can be calculated with

*Fax,mean= fv,0,mean· π · dh· *

*fv,0,mean*[N/mm2],*ρ [kg/m*3],*λ = /dh*[–],* [mm], dh*
*[mm], Fax _{,mean}*[N].

Figure 12 shows the fit of this equation with the density adjusted test results.

The use of the strength equation is restricted to:

### r

single rods glued-in parallel to the grain and loaded### r

slenderness ratios*λ = /dh*in the range of 7

*.5 ≤ λ ≤ 15*

### r

_{rod diameters d of 12 to 20 mm}### r

_{length}

_{}_{v}

_{= 5 · d}### r

edge distances*≥2.3·d*

### r

_{glulam made of Norway spruce or other coniferous}timber with similar properties and characteristic val-ues of density in the range of 350 to 500 kg/m3

_{.}

The proposed strength model only covers the ex-pected mean pull-out loads due to shear failure in the wood around the glued zone. In addition a control of the stresses in the steel bar and in the timber member (net cross-section) is necessary. In practice however the above pull-out strength formula only allows to calculate the maximum capacity of the joint for given geometri-cal parameters and for a certain timber density. Actually the joint should rather be designed in such a way that (ductile) steel failure occurs and (brittle) timber failure is prevented. Failure of the bond line or internal adhe-sive failure is to be prevented in any case in order to get ductile steel failure and optimal performance of the glued-in rod joint.

**5. Conclusions**

Based on the test results it can be stated, that for the used GSAR-system:

### r

_{the pull-out strength of rods bonded parallel to the}grain in glulam made of Norway spruce depends on the density of the timber around the anchoring zone. The influence of the density is clearly marked and can be covered by a power function

*ρc*

_{with an exponent}

*of c*= 0.6.

### r

_{the influence of the anchoring length}

*load values is marked and can be taken into account by an adjustment to the formulas based on*

_{ on ultimate}*−1/3*.

### r

_{an influence of the diameter dh}_{of the drill-hole on}

the pull-out strength could not be clearly evaluated.

### r

a dependence of ultimate loads on the slendernessra-tio*λ = /dh, which can be quantified byλ−1/3*could
be shown.

### r

with regard to optimal load transfer capacity from steel to timber, rods with smaller diameter should be given preference.**Acknowledgements The presented work was funded partly by**

the Swiss State Secretariat for Education and Research SER

within the framework of COST Action E34 ‘Bonding of Tim-ber’. The assistance of T. Strahm (sample logistics) and K. Weiss (mechanical testing) is gratefully acknowledged.

**References**

1. (2001) Proceedings of the International RILEM-Symposium on Joints in Timber Structures, Stuttgart, Germany 2. (1995) Proceedings of the CIB-W18 Meeting Twenty-Eight,

Copenhagen, Denmark

3. (1999) Proceedings of the CIB-W18 Meeting Thirty-Two, Graz, Austria

4. (2000) Proceedings of the CIB-W18 Meeting Thirty-Three, Delft, The Netherlands

5. (2001) Proceedings of the CIB-W18 Meeting Thirty-Four, Venice, Italy

6. Riberholt H (1988) Glued bolts in glulam – proposal for CIB code. Proceedings of the CIB-W18 Meeting Twenty-One, Parksville, Vancouver Island, Canada, Paper 21-7-2 7. M¨ohler K, Siebert W (1981) Glued-in rods,

Holzbau-Statik-Aktuell 6:4–6 (only available in German)

8. Aicher S, Gustafsson PJ, Wolf M (1999) Load displacement and bond strength of glued-in rods in timber influenced by adhesive, wood density, rod slenderness and diameter. Pro-ceedings of the International RILEM Symposium on Timber Engineering, Stockolm, Sweden, 10

9. ENV 1995-2 1997. Eurocode 5 – Design of timber structures (CEN, Bruxelles, 1997).

10. Gustafsson P-J, Serrano E, Aicher S, Johansson C-J (2001) A strength design equation for glued-in rods. Proceedings of the International RILEM Symposium on Joints in Timber Structures, Stuttgart, Germany, 323–332

11. Strahm T (2000) The GSA-system of anchorage: effi-cient and easy to design. Proceedings of the 32 SAH-Fortbildungskurs “Verbindungstechnik im Holzbau, Wein-felden, Switzerland, 165–169 (only available in German) 12. Ehlbeck J (1976) Tests on special nails for timber structures,

Holz als Roh- und Werkstoff 34(7):205–211 (only available in German)

13. Meierhofer U (1988) Screw withdrawal resistance and strength of spruce and fir. Holz als Roh- und Werkstoff 46(1):15–17 (only available in German)

14. G¨orlacher R (1990) Examination of old structural tim-ber: measurement of withdrawal resistance. bauen mit holz 92(12):904–908 (only available in German)

15. Werner H, Siebert W (1991) New investigations of nails in timber structures. Holz als Roh- und Werkstoff 49(5):191– 198 (only available in German)

16. Gerold M (1992) Compound of timber and threaded steel bars. Bautechnik 69(4):167–178 (only available in German) 17. Serrano E (2001) Glued-in rods for timber structures – an experimental study of softening behaviour. Materials and Structures 34:228–234

18. Kemmsies M (1999) Comparison of pull-out strengths of 12 adhesives for glued-in rods for timber structures. SP Re-port 20 (SP Swedish National Testing and Research Institute, 1999)

19. Bengtsson C, Johansson C-J (2000) Test methods for glued-in rods for timber structures. Proceedglued-ings of the CIB-W18 Meeting Thirty-Three, Delft, The Netherlands, Paper 33-7-8

20. Bernasconi A (2001) Behaviour of axially loaded glued-in rods – requirements and resistance, especially for spruce tim-ber perpendicular to the grain direction. Proceedings of the CIB-W18 Meeting Thirty-Four, Venice, Italy, Paper 34-7-6 21. Gerold M (1993) Application of threaded glued-in steel bolts with an applied load in direction of the pin. Bautechnik 70(10):603–613 (only available in German)

22. Gehri E (1996) Load transfer by means of steel bars. Proceed-ings of the 28 SAH-Fortbildungskurs “Brettschichtholz”, Weinfelden, Switzerland, 111–143 (only available in German)

23. Kangas J (2000) Capacity, fire resistance and gluing pattern of the rods in V-connections. Proceedings of the CIB-W18 Meeting Thirty-Three, Delft, The Netherlands, Paper 33-7-10

24. Gehri E (1997) Background paper on glued-in rods. Docu-ment 108 rev. (CEN, Bruxelles)

25. M¨ohler K, Hemmer K (1981) Glued-in rods. bauen mit holz 83(5):296–298 (only available in German)

26. Gehri E (2000) Re-investigation of classical joints. Proceed-ings of the 17 Dreil¨ander Holztagung Holz: Architecture – Research – Technology, Lucerne, Switzerland, 43–50 (only available in German)

27. Blass HJ, Laskewitz B (1999) Effect of spacing and edge distance on the axial strength of glued-in rods. Proceedings

of the CIB-W18 Meeting Thirty-Two, Graz, Austria, Paper 32-7-12

28. Bengtsson C, Johansson C-J (2001) Girod – glued-in rods for timber structures. Proceedings of the CIB-W18 Meeting Thirty-Four, Venice, Italy, Paper 34-7-8

29. Riberholt H (1986) Glued bolts in glulam. Proceedings of the CIB-W18 Meeting Nineteen, Florence, Italy, Paper 19-7-2 30. Fabris A (2001) Improved tensile strength parallel to the

grain of structural timber by means of a compound with threaded steel bars. phd thesis Nr. 14050, ETH Zurich, Switzerland (only available in German)

31. Gehri E (2001) Ductile behaviour and group effect of glued-in steel rods. Proceedglued-ings of the International RILEM Sym-posium on Joints in Timber Structures, Stuttgart, Germany, 333–342

32. EN 26891 (1991) Timber structures – joints made with mechanical fasteners: general principles for the de-termination of strength and deformation characteristics (CEN, Bruxelles)

33. Kangas J (1994) Joints of glulam structures based on glued-in ribbed steel rods. VTT Publication 196 (VTT, Helsglued-inki, Finland)

34. Del Senno M, Piazza M, Tomasi R (2004) Axial glued-in steel timber joints – experimental and numerical analysis, Holz als Roh- und Werkstoff 62:137–146

35. Deng JX, Moss PJ, Buchanan AH (1998) Glued bolts in glulam – an analysis of stress distribution. Proceedings of the 5th World Conference on Timber Engineering, Lausanne, Switzerland, 206–213